Upcoming SlideShare
×

# Block 9 agg specific gravity 13

2,248 views

Published on

3 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

Views
Total views
2,248
On SlideShare
0
From Embeds
0
Number of Embeds
2
Actions
Shares
0
120
0
Likes
3
Embeds 0
No embeds

No notes for slide
• The lecture will discuss aggregate specific gravities.
• The concept of volumetrics is a basic one that applies to all matter.
• Specific gravity is how much heavier an object compared to the weight of the same volume of water.
• Density is the specific gravity times the unit weight (mass) of water and relates mass to volume: for example, grams per cubic centimeter. Since the unit weight of water in units of 1 g/cm 3 , this term is sometimes left out of equations shown in test methods. Care needs to be taken if the units of the test are changed.
• This slide defines the mass and the volume used to calculate the bulk specific gravity (dry) of aggregates. G designates specific gravity. The subscripts indicate the material tested (s = stone) and the type of specific gravity (b=bulk). In this case, bulk is used because there is more than one component in the volume.
• This slide shows the mass and volumes used to determine the bulk specific gravity, ssd (saturated surface dry).
• This slide shows the mass and volume used to determine the apparent specific gravity.
• A phase diagram is usually used to represent relationships between mass and volume. The specific gravity of each component in the mixture is needed in order to determine the corresponding volume a given mass occupies. This slide shows a general two-phase diagram.
• The specific gravities of aggregates need to be determined separately for the fine and coarse fractions of either a stockpile or a blended material.
• This slide lists the general steps needed to determine the specific gravities of coarse aggregates.
• This photograph shows a sample of aggregate soaking (ready to test), a towel for drying, a spray bottle for pre-wetting the towel, the wire basket for obtaining the weight of SSD aggregate under water, and the water tank under the scale platform.
• The sample of coarse aggregate is being dried. Note the area of aggregate not being worked is covered with the towel so it will not dry out.
• These are the equations for calculating the bulk specific gravity (G sb ), bulk specific gravity saturated surface dry (G s, SSD ), apparent specific gravity (G sa ), and water absorption capacity. The denominator in all of the specific gravity equations is the mass of water displaced by the sample. Since 1 gram of water equals 1 cubic centimeter, this value also represents the volume of water displaced by the sample.
• These are the steps necessary for determining the specific gravity of the fine aggregate.
• A presoaked sample of fine aggregate is dried back to saturated surface dry condition using a gently moving warm current of air. In this case, a standard hair dryer is used. Saturated surface dry is determined using the cone test. An area is cleared in the center of the work area and the cone is filled to overflowing with the aggregate. The aggregate is then tamped down.
• The aggregate is considered to be saturated surface dry when the sand cone slumps when the brass form is removed.
• Once the saturated surface dry condition has been achieved, a 500 gram sample (weighed) is placed in a partially filled volumetric glass flask of known volume. The sample is then agitated until the foam and air bubbles have subsided. The flask is then filled with water up to the volumetric mark used for calibration and the mass of the pycnometer (flask), aggregate, and water recorded.
• These equations are similar to those used to determine the specific gravities of the coarse aggregate. Again, the denominator represents the volume of water displaced by the aggregate
• This slide is a review of the specific gravity variables introduced in this block.
• ### Block 9 agg specific gravity 13

1. 1. Senior/Graduate HMA Course Aggregate Specific GravitiesAggregates Aggregate Specific Gravities 1
2. 2. Volumetrics • All matter has mass and occupies space. • Volumetrics are the relationships between mass and volume • Superpave mix design based on aggregate and mixture volumetricsAggregates Aggregate Specific Gravities 2
3. 3. Specific Gravity, G • Ratio of the mass to volume of an object to that of water at the same temperature Mass Solid Volume Mass Water VolumeAggregates Aggregate Specific Gravities 3
4. 4. Densities • Density is the unit weight of a material • lb/ft3 or kg/m3 • Unit weight = γ w G γ w = 1.000 g/cm3 γ w = 62.4 lb/ft3 γ w = 1000 kg/m3 Bulk density means sample contains more than one mass and/or volumeAggregates Aggregate Specific Gravities 4
5. 5. Bulk Specific Gravity, Dry Mass, oven drySurface Voids Gsb = Vol of agg, + surface voids Vol. of water-perm. voidsAggregates Aggregate Specific Gravities 5
6. 6. Bulk Specific Gravity, SSD Mass, oven dry agg + mass water Gs, ssd = Vol of agg, + surface voids Vol. of water-perm. voids Surface VoidsAggregates Aggregate Specific Gravities 6
7. 7. Apparent Specific Gravity Mass, oven dry agg Gsa = Vol of aggAggregates Aggregate Specific Gravities 7
8. 8. Phase DiagramPhase: a change in state (e.g. solid, liquid, gas) V = (mass) / (Gs γ w) Volume Mass (Weight) Water permeable voids Aggregate SolidsAggregates Aggregate Specific Gravities 8
9. 9. Specific Gravity Tests for Aggregates • Two tests are needed • Coarse aggregate (retained on the 4.75 mm sieve) • Fine aggregate (passing the 4.75 mm sieve)Aggregates Aggregate Specific Gravities 9
10. 10. Coarse Aggregate Specific Gravity • ASTM C127 • Dry aggregate • Soak in water for 24 hours • Decant water • Use pre-dampened towel to get SSD condition • Determine mass of SSD aggregate in bucket • Determine mass under water • Dry to constant mass • Determine oven dry massAggregates Aggregate Specific Gravities 10
11. 11. Coarse Aggregate Specific GravityAggregates Aggregate Specific Gravities 11
12. 12. Coarse Aggregate Specific GravityAggregates Aggregate Specific Gravities 12
13. 13. Coarse Aggregate Specific Gravity Calculations • Gsb = A / (B - C) • A = mass oven dry • B = mass SSD • C = mass under water • Gs,SSD = B / (B - C) • Gsa = A / (A - C) • Water absorption capacity, % • Absorption % = [(B - A) / A] * 100Aggregates Aggregate Specific Gravities 13
14. 14. Fine Aggregate Specific Gravity• ASTM C128 • Dry aggregate • Soak in water for 24 hours • Spread out and dry to SSD • Add 500 g of SSD aggregate to pycnometer of known volume • Pre-filled with some water • Add more water and agitate until air bubble have been removed • Fill to line and determine the mass of the pycnometer, aggregate and water • Empty aggregate into pan and dry to constant mass • Determine oven dry massAggregates Aggregate Specific Gravities 14
15. 15. Fine Aggregate Specific GravityAggregates Aggregate Specific Gravities 15
16. 16. Fine Aggregate Specific GravityAggregates Aggregate Specific Gravities 16
17. 17. Fine Aggregate Specific GravityAggregates Aggregate Specific Gravities 17
18. 18. Fine Aggregate Specific Gravity Calculations• Gsb = A / (B + S - C) • A = mass oven dry • B = mass of pycnometer filled with water • C = mass pycnometer, SSD aggregate and water • S = mass SSD aggregate• Gs,SSD = S / (B + S - C)• Gsa = A / (B + A - C)• Water absorption capacity, % • Absorption % = [(S - A) / A] * 100Aggregates Aggregate Specific Gravities 18
19. 19. Summary of Terms • Gsb = Gravity stone bulk • Gsa = Gravity stone apparent • Gsb(ssd) = Gravity stone bulk (saturated surface dry) • γω = unit weight of waterAggregates Aggregate Specific Gravities 19
20. 20. QUESTIONS ?Aggregates Aggregate Specific Gravities 20